Active Standard ASTM A131 / A131M | Developed by Subcommittee: A01.02
Book of Standards Volume: 01.04
Historical (view previous versions of standard)
This specification covers structural steel plates, shapes, bars, and rivets for use in ship construction. Materials under this specification can be categorized as ordinary strength and higher strength. Plates in all thicknesses shall be normalized or thermo-mechanical control processed while shapes and bars in all thicknesses shall be heat treated and rolled. Heat analysis of ordinary strength structural steel shall be used to determine the required chemical composition for carbon, manganese, phosphorus, sulfur, nickel, chromium, molybdenum, silicon, and copper. Same analysis shall be used to higher strength structural steel to determine the required chemical composition for carbon, manganese, phosphorus, sulfur, silicon, vanadium, aluminum, titanium, nickel, chromium, molybdenum, silicon, copper, nickel, and niobium. Materials shall conform to the required metallurgical structure which shall be evaluated by determining the average grain size. Mechanical properties such as elongation and toughness shall be evaluated using tension test and Charpy V-notch impact test.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers structural steel plates, shapes, bars, and rivets intended primarily for use in ship construction.
1.2 Material under this specification is available in the following categories:
1.2.1 Ordinary Strength—Grades A, B, D, and E with a specified minimum yield point of 34 ksi [235 MPa], and
1.2.2 Higher Strength—Grades AH, DH, EH, and FH with a specified minimum yield point of 46 ksi [315 MPa], 51 ksi [350 MPa], or 57 ksi [390 MPa].
1.3 Shapes and bars are normally available as Grades A, AH32, and AH36. Other grades may be furnished by agreement between the purchaser and the manufacturer.
1.4 The maximum thickness of products furnished under this specification is 4 in. [100 mm] for plates and 2 in. [50 mm] for shapes and bars.
1.5 When the steel is to be welded, it is presupposed that a welding procedure suitable for the grade of steel and intended use or service will be utilized. See Appendix X3 of Specification A6/A6M for information on weldability.
1.6 The values stated in either inch-pound units or SI units are to be regarded separately as the standard. Within the text, the SI units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with this specification.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A6/A6M Specification for General Requirements for Rolled Structural Steel Bars, Plates, Shapes, and Sheet Piling
A370 Test Methods and Definitions for Mechanical Testing of Steel Products
E112 Test Methods for Determining Average Grain Size
ICS Number Code 47.020.05 (Materials and components for shipbuilding)
UNSPSC Code 30260000(Structural materials)